# Lab 8 Tensile Testing

```Lab 8: Tensile Testing
1. INTRODUCTION
The mechanical properties of materials are determined by performing carefully
designed laboratory experiments that replicate as nearly as possible the service conditions.
In real life, there are many factors involved in the nature in which loads are applied on a
material. The following are some common examples of modes in which loads might be
applied: tensile, compressive, and shear. These properties are important in materials
selections for mechanical design. Other factors that often complicate the design process
include temperature and time factors.
The topic of this lab is confined to the tensile
property of polymers. Figure 1 shows a tensile testing
machine similar to the one used in this lab. This test
is a destructive method, in which a specimen of a
standard shape and dimensions (prepared according
to ASTM D 638: standard test method for tensile
properties of plastics) is subjected to an axial load.
During a typical tensile experiment, a dog-bone
shaped specimen is gripped at its two ends and is
pulled to elongate at a determined rate to its
breakpoint; a highly ductile polymer may not reach
its breakpoint. The tensile tester used in this lab is
manufactured by Instron (model 5569).
It has a
maximum load of 2 or 50 kN and a variable pulling rate.
The setup of the experiment could be changed to
Figure 1. A photograph of a tensile
machine Instron 5569
accommodate different types of mechanical testing, according to the ASTM standard (e.g.
compression test, etc).
For analytical purposes, a plot of stress (σ) versus strain (ε) is constructed during
a tensile test experiment, which can be done automatically on the software provided by
the instrument manufacturer. Stress, in the metric system, is usually measured in N/m2 or
1
Pa, such that 1 N/m2 = 1 Pa. From the experiment, the value of stress is calculated by
dividing the amount of force (F) applied by the machine in the axial direction by its
cross-sectional area (A), which is measured prior to running the experiment.
Mathematically, it is expressed in Equation 1. The strain values, which have no units, can
be calculated using Equation 2, where L is the instantaneous length of the specimen and
L0 is the initial length.

F
A
(Equation 1)

L  L0
L0
(Equation 2)
A typical stress-strain curve would look like Figure 2. The stress-strain curve
shown in Figure 2 is a textbook example of a stress-strain curve. In reality, not all stressstrain curves perfectly resemble the one shown in Figure 2. This stress-strain curve is
typical for ductile metallic elements. Another thing to take note is that Figure 2 shows an
“engineering stress-strain” curve. When a material reaches its ultimate stress strength of
the stress-strain curve, its cross-sectional area reduces dramatically, a term known as
necking.
When
the
computer software plots the
stress-strain
assumes
curve,
that
the
it
cross
sectional area stays constant
throughout the experiment,
even
during
necking,
therefore causing the curve
to slope down. The “true”
stress-strain curve could be
constructed
directly
by
installing a “gauge,” which
Figure 2. Various regions and points on the stress-strain curve.
measures the change in the cross sectional area of the specimen throughout the
experiment.
2
Theoretically, even without measuring the cross-sectional area of the specimen
during the tensile experiment, the “true” stress-strain curve could still be constructed by
assuming that the volume of the material stays the same. Using this concept, both the true
stress (σT) and the true strain (εT) could be calculated using Equations 3 and 4,
respectively. The derivation of these equations is beyond the scope of this lab report.
equations, L0 refers to the initial length of the specimen, L refers to the instantaneous
length and σ refers to the instantaneous stress.
T  
L
L0
(Equation 3)
 L

 L0 
(Equation 4)
 T  ln 
Figure 2 also shows that a stress-strain curve is divided into four regions: elastic,
yielding, strain hardening (commonly occurs in metallic materials), and necking. The
area under the curve represents the amount of energy needed to accomplish each of these
“events.” The total area under the curve (up to the point of fracture) is also known as the
modulus of toughness. This represents the amount of energy needed to break the sample,
which could be compared to the impact energy of the sample, determined from impact
tests. The area under the linear region of the curve is known as the modulus of resilience.
This represents the minimum amount of energy needed to deform the sample.
The linear region of the curve of Figure 2, which is called the elastic region (past
this region, is called the plastic region), is the region where a material behaves elastically.
The material will return to its original shape when a force is released while the material is
in its elastic region. The slope of the curve, which can be calculated using Equation 5, is a
constant and is an intrinsic property of a material known as the elastic modulus, E. In
metric units, it is usually expressed in Pascals (Pa).
E


(Equation 5)
3
Figure 3(a) shows typical stress-strain curves of polymers. The figure shows that
materials that are hard and brittle do not deform very much before breaking and have
very steep elastic moduli.
The mechanical property of polymers generally depends on their degree of
crystallinity, molecular weights and glass transition temperature, Tg. Highly crystalline
polymeric materials with a Tg above the room temperature are usually brittle, and vice
versa. When a semi-crystalline polymer undergoes a tensile test, the amorphous chains,
will become aligned. This is usually evident for transparent and translucent materials,
which become opaque upon turning crystalline. Figure 3(b) shows a diagram showing the
mechanical property of some common polymers.
(a)
(b)
Figure 3. (a) A plot of stress-strain curves of typical polymeric materials. (b) A summary diagram of
the properties of common polymers.
4
2. EXPERIMENTAL PROCEDURE
Important! Make sure you wear safety glasses before starting any operation. Your eyes
could be hurt by a broken piece of polymer. Also wear gloves to protect against any
residue on the machine and samples.
2.1 Specimen Preparation
The polymer specimens were injection-molded into dog-bone shapes. Their dimensions
were determined according to the ASTM D 638 standard mentioned earlier in the
introduction.
(1) Measure the thickness, width and gage length of polymer samples in mm. These
dimensions should be approximately the same for each sample.
(2) Also make note of any sample defects (e.g. impurities, air bubbles, etc.).
The following samples will be tested:
1) Polypropylene (PP), polystyrene (PS), polylactic acid (biopolymer), high density
polyethylene (HDPE), and Dynaflex for analysis of mechanical properties.
2) Polystyrene: to compare effects of feeding direction on mechanical properties.
3) Polypropylene: to analyze effects of strain rate on mechanical properties.
2.2 Bluehill Software Setup
1) Turn on the tensile test machine. The switch is located on the right side of the
machine. Also turn on the video extensometer.
(2) Go to the desktop and double-click on the “Bluehill” icon.
(3) On the main page, select Test to start a new sample. Name your test and click Browse
to select the folder you would like to save it in. Click next.
(4) Choose which method you would like to use. Create and save a new method if
needed.
(5) Method set up: Save after any changes are made.

General: used for display purposes
5

Specimen: specifies sample dimensions and parameters. A dogbone
sample is used for tensile testing. Select rectangular, and specify the
width, thickness and gauge length of the sample. The gauge length is the
distance between the clamps before starting the test.

Control: describes the actual test. Select extension for mode of
displacement, then specify the rate of extension. Most use 5 mm/min or
50 min/mm, depending on if you want a slow or fast test.

End of Test: identifies the criteria for the end of the test. A large load
drop is experienced when sample failure occurs. For this test, when the
sample load drops by a certain percentage of the peak load, the machine
will stop.

Data: specifies if the data is acquired manually or automatically, while the
strain tab recognizes whether the strain is measured from the video
extensimeter or the extension.

Results and Graphs: select what data is shown and how it is displayed.
2.3 Instrument Setup
(1) Make sure the proper load cell is installed, either 2 kN or 50 kN depending on the
load range and sensitivity of the sample. To switch load cells, make sure the machine
is off. Unscrew the bolts and remove using the handle. Make sure to plug the new
load cell into the port behind the machine.
(2) Calibrate the load cell by clicking on the button in the upper right hand corner. Make
sure all loads are removed from the load cell and click calibrate.
(3) Install the correct type of clamps for the testing. For tensile testing, 5kN or 50kN
samples can be used. Install the clamps using the pins. Also install height brackets if
needed. Zero the load once the clamps are installed.
(4) Press the up and down arrows on the controller until the clamps are just touching.
Press the reset gauge length button at the top of the screen to zero the position of the
clamps.
(5) Use the up and down arrows until the clamps are about 100 mm apart. This is a
typical gauge length for the dog bone samples.
6
(6) Place the polymer sample between the grips of both the tensile test machine. While
holding the sample vertically with one hand, use another hand to turn the handle of
the top grip in the closing direction as tightly as possible.
(The specimen should be gripped such that the two ends of the specimen are covered
by the grip, approximately 3 mm away from its gage-length. It is important that the
specimens are tightly gripped onto the specimen grips to prevent slipping, which will
otherwise result in experimental errors. )
(8) Make sure that the specimen is vertically aligned, if not a torsional force, rather than
axial force, will result.
(9) Turn the bottom handle in the “close” direction as tightly as possible. Visually verify
that the sample is gripped symmetrically at its two ends.
(10)Zero the extension by pushing zero extension button at the top of the screen. Also
zero the load if needed. Wait for a few seconds to let the computer return its value to
zero.
2.4 Tensile Test
(1) Enter geometry of the sample before starting.
(2) Click on the Start button. Both the upper and bottom grips will start moving in
opposite directions according to the specified pulling rate. Observe the experiment at
a safe distance (about 1.5 meters away) at an angle and take note of the failure mode
when the specimen fails.
(NOTE: Be sure to wear safety glasses. Do not come close to equipment when the
tensile test is running).
(3) A plot of tensile stress (MPa) versus tensile strain (mm/mm) will be generated in realtime during the experiment.
2.6 End of Test
(1) The machine will stop automatically when the sample is broken.
(2) Press the “Return” button on the digital controller. Both the upper and lower grips
will be returned to their original positions automatically.
(3) Turn the two handles in the open directions to remove the sample
7
(4) Repeat the previous steps for any additional tests.
(5) When finished, save your file and click Finish. This will export your data into a PDF
and individual data files.
(6) Clean up any broken fragments from the specimens.
(7) Turn off the machine and exit the program when finished.
3. ASSIGNMENTS

Graph PP (50 mm/mm extension), PS (2 feed inputs), PLA, HDPE and Dynaflex
results using raw data files. There should be two tests for each polymer, but just pick
one to graph. Construct the true stress-strain curves for each polymer (hint: use
Equations (3) and (4) provided in the Introduction section).

Calculate Young’s Modulus for each material and testing condition and compare
experimental values with literature values.

Discuss any differences in mechanical behavior between the polymers (use pictures!)

Analyze the fracture modes of each sample (ductile fracture, brittle fracture, or
intermediate fracture mode).

Using the data for polypropylene, discuss the effects of strain rate on the mechanical
behavior of the polymers.

Using the data for polystyrene, compare effects of feed direction on the mechanical
behavior.

Explain any unexpected results.
8
```